nucleation kinetics, growth and characterization studies ... nucleation kinetics, growth and...
Post on 07-Mar-2020
Embed Size (px)
ISSN: 0973-4945; CODEN ECJHAO E-Journal of Chemistry
http://www.e-journals.net 2009, 6(3), 871-879
Nucleation Kinetics, Growth and Characterization
Studies of a Diamagnetic Crystal-Zinc Sulphate
R. KANAGADURAI#, R. DURAIRAJAN¶*, R. SANKAR§, G. SIVANESAN, S. P. ELANGOVAN¶ and R. JAYAVEL§
#Department of Physics, R.S. Govt. College, Thanjavur-613 005, India. ¶Department of Chemistry, R.S.Govt. College, Thanjavur-613 005, India.
§Crystal Growth Centre, Anna University, Chennai-600 025, India.
J.J.College of Arts and Science, Pudukkottai-622 404, Tamil Nadu, India. firstname.lastname@example.org
Received 31 October 2008; Revised 13 January 2009; Accepted 16 January 2009
Abstract: Solubility, metastable zone width and induction period measurements have been performed on zinc sulphate heptahydrate (ZSHH). Interfacial tension values determined from induction period measurements have been used for the evaluation of the nucleation parameters such as radius of critical nucleus and the free energy of formation of critical nucleus. ZSHH crystallizes in the orthorhombic structure. Crystals of diamagnetic zinc sulphate heptahydrate have been grown by temperature lowering solution growth technique with the optimized growth parameters. The as-grown ZSHH crystals were characterized by the powder X-ray diffraction, UV-VIS absorption and transmittance, FT-IR absorption, TG-DTA, microhardness and etching studies.
Keywords: ZSHH, Nucleation studies, Induction period, Solubility, Diamagnetic.
Diamagnetic Zinc sulphate heptahydrate finds wide applications in solar systems for solar energy storage, in making lithophone, in coagulation baths for rayon, in electrolyte for zinc plating, in medicine as an astringent and emetic and used to supply zinc in animal feeds, fertilizers, agricultural sprays, as a moderant in dyeing, as a preservative for skins and leather. But quite often inadequate transparency, poor optical quality and inability to grow large size crystals have impeded the use of single crystals of diamagnetic materials in practical device application. Growth of bulk single crystals of these materials has been a subject of perennial concern in order to use them for device application.
872 R. KANAGADURAI et al.
Single crystals of ZSHH were grown in very small size by silica gel method1. In order to optimize the growth parameters for growing bulk crystals, a systematic investigation has been made on the experimental determination of solubility, metastable zone width and induction period values. The interfacial energy has been estimated using the experimentally determined induction period values. Using the optimized growth parameters bulk crystals of size 70 x 11 x 4 mm3 have been grown. Optical, thermal properties, mechanical strength and surface analysis of ZSHH crystal have also been studied.
The calculated amounts of the ZSHH salts were dissolved in deionized water. This solution was heated and kept for slow evaporation to dryness at room temperature. The purity of the salt was improved by successive recrystallisation process. The solubility of ZSHH was determined for four different temperatures, 30, 35, 40, and 45 ºC. by dissolving the solute in deionized water in an air tight container maintained at a constant temperature with stirring. After attaining saturation, the equilibrium concentration of the solute was analyzed gravimetrically. The same procedure was repeated and the solubility curves for different temperatures were drawn. Figure (1) shows the solubility curve for zinc sulphate heptahydrate at different temperatures.
Figure 1. Solubility of ZSHH as a function temperature in aqueous solution.
Metastable zone width and induction period measurements
Saturated solution of zinc sulphate heptahydrate was prepared from solubility experiment. The metastable zone width was measured by the conventional polythermal method2,3. The studies were carried out in a constant temperature bath controlled to an accuracy of ±0.05 °C, provided with a cryostat for cooling below room temperature. A constant volume of 150 mL of the solution was used for all the experiments. The solution was heated to 5 °C above the supersaturation temperature for homogenization and was kept at the superheated temperature for one hour before cooling. It was continuously stirred using a motorized stirrer to ensure homogeneous concentration and temperature throughout the entire volume of the solution. The temperature of the bath was reduced at a rate of 0.5 oC per minute with continuous stirring after the stabilization. The temperature at which the first speck of a particle appeared was noted. The first speck of crystal obtained is taken as critical nucleus. The time taken for
28 30 32 34 36 38 40 42 44 46
/ 5 0
Nucleation Kinetics, Growth and Characterization Studies 873
the formation of the critical nucleus is called induction period (τ) and the induction period of zinc sulphate heptahydrate was measured by means of isothermal method. Repeated trials were carried out to ensure reproducibility. It was observed that metastable zone width decrease with increase of temperature as shown in the Figure 2.
Figure 2. Meta stable zone width as a function of temperature in aqueous solution.
Interfacial tension of the crystal and solution interface is an important parameter involved in the theory of nucleation and growth kinetics. In the present investigation, in order to estimate the critical nucleation parameters, the interfacial tension has been calculated on the basis of the classical theory of homogeneous nucleation4-6.
The interfacial tension of the solid relative to this solution has been calculated from the relation
τ σ = (1)
Where σ is the interfacial tension, V is the molar volume of the crystal, N is the Avogadro's number, R is the gas constant and S is the relative supersaturation (S=C/C*) where C is the actual concentration and C* is the equilibrium concentration. Figure (3) shows the variation of induction period as a function of supersaturation ratio for various temperatures. According to the classical homogeneous nucleation theory the free energy required to form a spherical nucleus is given by
σππ 23 4 3
4 rGrG v +∆=∆ (2)
Where ∆Gv is the energy change per unit volume, r is the radius of the nucleus. At the critical state, the free energy of formation obeys the condition that d (∆G/dr) = 0. Hence the radius of the critical nucleus is expressed as
σ2 * , where vSkTGv /ln−=∆ , where V is
the molar volume, S is the relative super saturation. Hence,
60 70 80 90 100 110 120 130
p e a rt
Concentration (g/50ml)Concentration, g/ 50 mL
, 0 C
874 R. KANAGADURAI et al.
The critical free energy is given by
Figure 3. Variation of induction period with super saturation ratio for ZSHH solution.
ZSHH possesses the interfacial energy ranging from 1.7049 to 3.5368 mJ/m2. The energy of formation (∆G*) and radius (r*) of the critical nucleus of ZSHH were found to be from 2.8125 to 2.0149 kJ/mol and from 1.985 nm to 1.1665 respectively at different supersaturation level. Experimentally determined values of induction period, interfacial tension, critical nucleus and critical free energy of formation of ZSHH crystal are shown in Table 1. The interfacial tension increases with supersaturation as shown in Figure 4.
Table 1. Experimentally determined values of induction period, interfacial tension, critical nucleus and critical free energy of formation of zinc sulphate hepta hydrate crystal.
Induction period, sec
Interfacial tension σ, mJ/m2
Critical nucleus r*, nm
Critical free energy of formation ∆G* kJ/mol
1.1 600 1.7049 1.985 2.8125 1.2 280 2.5182 1.5327 2.4769 1.3 175 3.1176 1.3186 2.2697
1.4 98 3.5368 1.1665 2.0149
Bulk crystal growth
To grow bulk crystal, the supersaturated solution of zinc sulphate heptahydrate was kept in a constant temperature bath with an accuracy of ±0.01º C at 45ºC. The seed crystal of ZSHH, obtained by slow evaporation method, was suspended in the supersaturated solution. The temperature of the bath was reduced at the rate of 0.05ºC per day. Good transparent sing